LMucko/crystallography-open-database huggingface dataset:
Lattice parameters of magnesium alloys
Busk, R.S.; Transactions of the American Institute of Mining, Metallurgical and Petroleum Engineers 188 (1950) 1460–1464; doi:

data_1523361
_publ_section_title
;
 Lattice parameters of magnesium alloys
;
_journal_name_full
;
Transactions of the American Institute of Mining, Metallurgical and Petroleum 
Engineers
;
_journal_page_first              1460
_journal_page_last               1464
_journal_volume                  188
_journal_year                    1950
_chemical_formula_sum            'Hg0.012 Mg0.988'
_chemical_name_systematic        '(Hg0.012 Mg0.988)'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   3.2042
_cell_length_b                   3.2042
_cell_length_c                   5.2023
_cell_volume                     46.256
_citation_journal_id_ASTM        TAIMAF
_cod_data_source_file            Busk_TAIMAF_1950_636.cif
_cod_data_source_block           Hg0.012Mg0.988
_cod_original_cell_volume        46.2557
_cod_database_code               1523361
Magnetic order in rare-earth intermetallic compounds
Cable, J.W.; Koehler, W.C.; Wollan, E.O.; Physical Review, Section A (133,1964-188,1969) 136 (1964) 240–242; doi:

data_1523362
_publ_section_title
;
 Magnetic order in rare-earth intermetallic compounds
;
_journal_name_full
'Physical Review, Section A (133,1964-188,1969)'
_journal_page_first              240
_journal_page_last               242
_journal_volume                  136
_journal_year                    1964
_chemical_formula_sum            'Ga Tb'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.33
_cell_length_b                   10.9
_cell_length_c                   4.09
_cell_volume                     193.036
_citation_journal_id_ASTM        PRVAAH
_cod_data_source_file            Cable_PRVAAH_1964_365.cif
_cod_data_source_block           Ga1Tb1
_cod_original_cell_volume        193.0357
_cod_original_formula_sum        'Ga1 Tb1'
_cod_database_code               1523362
Magnetization studies of the Heusler alloys Ni2 Mnx V1-x Sn and Ni2 Mnx Cr1-x Sn
Campbell, C.C.M.; Stager, C.V.; Canadian Journal of Physics 54 (1976) 2197–2203; doi:

data_1523363
_publ_section_title
;
 Magnetization studies of the Heusler alloys Ni2 Mnx V1-x Sn and Ni2 Mnx
 Cr1-x Sn
;
_journal_name_full               'Canadian Journal of Physics'
_journal_page_first              2197
_journal_page_last               2203
_journal_volume                  54
_journal_year                    1976
_chemical_formula_sum            'Mn0.2 Ni Sn0.5 V0.3'
_chemical_name_systematic        '(Mn0.2 Sn0.5 V0.3) Ni'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   6.054
_cell_length_b                   6.054
_cell_length_c                   6.054
_cell_volume                     221.885
_citation_journal_id_ASTM        CJPHAD
_cod_data_source_file            Campbell_CJPHAD_1976_1137.cif
_cod_data_source_block           Mn0.2Ni1Sn0.5V0.3
_cod_original_cell_volume        221.8846
_cod_original_formula_sum        'Mn0.2 Ni1 Sn0.5 V0.3'
_cod_database_code               1523363
Magnetization studies of the Heusler alloys Ni2 Mnx V1-x Sn and Ni2 Mnx Cr1-x Sn
Campbell, C.C.M.; Stager, C.V.; Canadian Journal of Physics 54 (1976) 2197–2203; doi:

data_1523364
_publ_section_title
;
 Magnetization studies of the Heusler alloys Ni2 Mnx V1-x Sn and Ni2 Mnx
 Cr1-x Sn
;
_journal_name_full               'Canadian Journal of Physics'
_journal_page_first              2197
_journal_page_last               2203
_journal_volume                  54
_journal_year                    1976
_chemical_formula_sum            'Mn0.2 Ni Sn0.5 Ti0.3'
_chemical_name_systematic        '(Mn0.2 Sn0.5 Ti0.3) Ni'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   6.098
_cell_length_b                   6.098
_cell_length_c                   6.098
_cell_volume                     226.758
_citation_journal_id_ASTM        CJPHAD
_cod_data_source_file            Campbell_CJPHAD_1976_1138.cif
_cod_data_source_block           Mn0.2Ni1Sn0.5Ti0.3
_cod_original_cell_volume        226.7578
_cod_original_formula_sum        'Mn0.2 Ni1 Sn0.5 Ti0.3'
_cod_database_code               1523364
High-pressure synthesis of beta-W type Nb3 Te
Cannon, J.F.; Lawson, A.C.jr.; Robertson, D.L.; Hall, H.T.; Journal of Physics and Chemistry of Solids 35 (1974) 1181–1182; doi:

data_1523365
_publ_section_title
;
 High-pressure synthesis of beta-W type Nb3 Te
;
_journal_name_full               'Journal of Physics and Chemistry of Solids'
_journal_page_first              1181
_journal_page_last               1182
_journal_volume                  35
_journal_year                    1974
_chemical_formula_sum            'Nb3 Te'
_space_group_IT_number           223
_symmetry_space_group_name_Hall  '-P 4n 2 3'
_symmetry_space_group_name_H-M   'P m -3 n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.261
_cell_length_b                   5.261
_cell_length_c                   5.261
_cell_volume                     145.615
_citation_journal_id_ASTM        JPCSAW
_cod_data_source_file            Cannon_JPCSAW_1974_1408.cif
_cod_data_source_block           Nb3Te1
_cod_original_cell_volume        145.6146
_cod_original_formula_sum        'Nb3 Te1'
_cod_database_code               1523365
Synthesis of lanthanide-iron Laves phases at high pressures and temperatures
Cannon, J.F.; Robertson, D.L.; Hall, H.T.; Materials Research Bulletin 7 (1972) 5–12; doi:

data_1523366
_publ_section_title
;
 Synthesis of lanthanide-iron Laves phases at high pressures and
 temperatures
;
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              5
_journal_page_last               12
_journal_volume                  7
_journal_year                    1972
_chemical_formula_sum            'Fe2 Yb'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   7.239
_cell_length_b                   7.239
_cell_length_c                   7.239
_cell_volume                     379.346
_citation_journal_id_ASTM        MRBUAC
_cod_data_source_file            Cannon_MRBUAC_1972_124.cif
_cod_data_source_block           Fe2Yb1
_cod_original_cell_volume        379.3462
_cod_original_sg_symbol_Hall     '-F 4vw 2vw 3 (x+1/8,y+1/8,z+1/8)'
_cod_original_formula_sum        'Fe2 Yb1'
_cod_database_code               1523366
Effect of high pressure on the structures of A B3-type layered compounds
Cannon, J.F.; Materials Research Society Symposia Proceedings 22 (1984) 113–116; doi:

data_1523367
_publ_section_title
;
 Effect of high pressure on the structures of A B3-type layered compounds
;
_journal_name_full
'Materials Research Society Symposia Proceedings'
_journal_page_first              113
_journal_page_last               116
_journal_volume                  22
_journal_year                    1984
_chemical_formula_sum            'Fe3 Sn'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.873
_cell_length_b                   3.873
_cell_length_c                   3.873
_cell_volume                     58.095
_citation_journal_id_ASTM        MRSPDH
_cod_data_source_file            Cannon_MRSPDH_1984_68.cif
_cod_data_source_block           Fe3Sn1
_cod_original_cell_volume        58.0955
_cod_original_formula_sum        'Fe3 Sn1'
_cod_database_code               1523367
Die Struktur von Pt7 Zn12
Carl, W.; Schubert, K.; Journal of the Less-Common Metals 19 (1969) 279–283; doi:

data_1523368
_publ_section_title
;
 Die Struktur von Pt7 Zn12
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              279
_journal_page_last               283
_journal_volume                  19
_journal_year                    1969
_chemical_formula_sum            'Pt7 Zn12'
_space_group_IT_number           55
_symmetry_space_group_name_Hall  '-P 2 2ab'
_symmetry_space_group_name_H-M   'P b a m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   28.79
_cell_length_b                   6.94
_cell_length_c                   2.76
_cell_volume                     551.455
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Carl_JCOMAH_1969_1886.cif
_cod_data_source_block           Pt7Zn12
_cod_original_cell_volume        551.4552
_cod_database_code               1523368
Strukturuntersuchungen in einigen zu T(4)-T(9) homologen und quasihomolgen Legierungssystemen
Carl, W.; Schubert, K.; Zeitschrift fuer Metallkunde 55 (1964) 704–710; doi:

data_1523369
_publ_section_title
;
 Strukturuntersuchungen in einigen zu T(4)-T(9) homologen und
 quasihomolgen Legierungssystemen
;
_journal_name_full               'Zeitschrift fuer Metallkunde'
_journal_page_first              704
_journal_page_last               710
_journal_volume                  55
_journal_year                    1964
_chemical_formula_sum            'Pt Zr'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.31
_cell_length_b                   3.31
_cell_length_c                   3.31
_cell_volume                     36.265
_citation_journal_id_ASTM        ZEMTAE
_cod_data_source_file            Carl_ZEMTAE_1964_1887.cif
_cod_data_source_block           Pt1Zr1
_cod_original_cell_volume        36.26469
_cod_original_formula_sum        'Pt1 Zr1'
_cod_database_code               1523369
Thorium-columbium and thorium-titanium alloy systems
Carlson, O.N.; Lunt, H.E.; Dickinson, J.M.; Wilhelm, H.A.; Transactions of the American Institute of Mining, Metallurgical and Petroleum Engineers 206 (1956) 132–136; doi:

data_1523370
_publ_section_title
;
 Thorium-columbium and thorium-titanium alloy systems
;
_journal_name_full
;
Transactions of the American Institute of Mining, Metallurgical and Petroleum 
Engineers
;
_journal_page_first              132
_journal_page_last               136
_journal_volume                  206
_journal_year                    1956
_chemical_formula_sum            'Nb0.035 Th0.965'
_chemical_name_systematic        '(Nb0.035 Th0.965)'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.086
_cell_length_b                   5.086
_cell_length_c                   5.086
_cell_volume                     131.562
_citation_journal_id_ASTM        TAIMAF
_cod_data_source_file            Carlson_TAIMAF_1956_1410.cif
_cod_data_source_block           Nb0.035Th0.965
_cod_original_cell_volume        131.5616
_cod_database_code               1523370
The yttrium-lead alloy system
Carlson, O.N.; Schmidt, F.A.; Diesburg, D.E.; Transactions of the American Society for Metals 60 (1967) 119–124; doi:

data_1523371
_publ_section_title
;
 The yttrium-lead alloy system
;
_journal_name_full
'Transactions of the American Society for Metals'
_journal_page_first              119
_journal_page_last               124
_journal_volume                  60
_journal_year                    1967
_chemical_formula_sum            'Pb2 Y'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.55
_cell_length_b                   16.46
_cell_length_c                   4.45
_cell_volume                     333.274
_citation_journal_id_ASTM        TASEA7
_cod_data_source_file            Carlson_TASEA7_1967_1714.cif
_cod_data_source_block           Pb2Y1
_cod_original_cell_volume        333.2738
_cod_original_formula_sum        'Pb2 Y1'
_cod_database_code               1523371
The yttrium-lead alloy system
Carlson, O.N.; Schmidt, F.A.; Diesburg, D.E.; Transactions of the American Society for Metals 60 (1967) 119–124; doi:

data_1523372
_publ_section_title
;
 The yttrium-lead alloy system
;
_journal_name_full
'Transactions of the American Society for Metals'
_journal_page_first              119
_journal_page_last               124
_journal_volume                  60
_journal_year                    1967
_chemical_formula_sum            'Pb4 Y5'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.994
_cell_length_b                   15.1
_cell_length_c                   8.241
_cell_volume                     994.766
_citation_journal_id_ASTM        TASEA7
_cod_data_source_file            Carlson_TASEA7_1967_1717.cif
_cod_data_source_block           Pb4Y5
_cod_original_cell_volume        994.7662
_cod_database_code               1523372
Crystal structure refinement of delta-Ho Ga3
Carnasciali, M.M.; Franceschi, E.; Cirafici, S.; Journal of the Less-Common Metals 81 (1981) 115–119; doi:

data_1523373
_publ_section_title
;
 Crystal structure refinement of delta-Ho Ga3
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              115
_journal_page_last               119
_journal_volume                  81
_journal_year                    1981
_chemical_formula_sum            'Ga3 Ho'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   6.084
_cell_length_b                   6.084
_cell_length_c                   14.061
_cell_volume                     450.739
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Carnasciali_JCOMAH_1981_167.cif
_cod_data_source_block           Ga3Ho1
_cod_original_cell_volume        450.7391
_cod_original_formula_sum        'Ga3 Ho1'
_cod_database_code               1523373
Structure cristalline de la pretendue variete beta des sulfures de terres rares de composition Pr10 S14 O
Carre, D.; Laruelle, P.; Besancon, P.; Comptes Rendus Hebdomadaires des Seances de l'Academie des Sciences, Serie C, Sciences Chimiques (1966-) 270 (1970) 537–539; doi:

data_1523374
_publ_section_title
;
 Structure cristalline de la pretendue variete beta des sulfures de terres
 rares de composition Pr10 S14 O
;
_journal_name_full
;
Comptes Rendus Hebdomadaires des Seances de l'Academie des Sciences, Serie C, 
Sciences Chimiques (1966-)
;
_journal_page_first              537
_journal_page_last               539
_journal_volume                  270
_journal_year                    1970
_chemical_formula_sum            'O Pr10 S14'
_chemical_name_systematic        'Pr10 O S14'
_space_group_IT_number           142
_symmetry_space_group_name_Hall  '-I 4bd 2c'
_symmetry_space_group_name_H-M   'I 41/a c d :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   15.1
_cell_length_b                   15.1
_cell_length_c                   20.05
_cell_volume                     4571.600
_citation_journal_id_ASTM        CHDCAQ
_cod_data_source_file            Carre_CHDCAQ_1970_205.cif
_cod_data_source_block           O1Pr10S14
_cod_original_cell_volume        4571.601
_cod_original_formula_sum        'O1 Pr10 S14'
_cod_database_code               1523374
The equilibrium diagram of the system Mo-Ni
Casselton, R.E.W.; Hume-Rothery, W.; Journal of the Less-Common Metals 7 (1964) 212–221; doi:

data_1523375
_publ_section_title
;
 The equilibrium diagram of the system Mo-Ni
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              212
_journal_page_last               221
_journal_volume                  7
_journal_year                    1964
_chemical_formula_sum            'Mo1.08 Ni2.92'
_chemical_name_systematic        '(Mo1.08 Ni2.92)'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.6373
_cell_length_b                   3.6373
_cell_length_c                   3.6373
_cell_volume                     48.121
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Casselton_JCOMAH_1964_1229.cif
_cod_data_source_block           Mo1.08Ni2.92
_cod_original_cell_volume        48.1213
_cod_database_code               1523375
The equilibrium diagram of the system Mo-Ni
Casselton, R.E.W.; Hume-Rothery, W.; Journal of the Less-Common Metals 7 (1964) 212–221; doi:

data_1523376
_publ_section_title
;
 The equilibrium diagram of the system Mo-Ni
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              212
_journal_page_last               221
_journal_volume                  7
_journal_year                    1964
_chemical_formula_sum            'Mo0.984 Ni0.016'
_chemical_name_systematic        '(Mo0.984 Ni0.016)'
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.1441
_cell_length_b                   3.1441
_cell_length_c                   3.1441
_cell_volume                     31.081
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Casselton_JCOMAH_1964_1233.cif
_cod_data_source_block           Mo0.984Ni0.016
_cod_original_cell_volume        31.08057
_cod_database_code               1523376
Magnetic properties and structures of equiatomic rare earth-platinum compounds R Pt (R= Gd, Tb, Dy, Ho, Fr, Tm)
Castets, A.; Gignoux, D.; Gomez-Sal, J.C.; Journal of Solid State Chemistry 31 (1980) 197–207; doi:

data_1523377
_publ_section_title
;
 Magnetic properties and structures of equiatomic rare earth-platinum
 compounds R Pt (R= Gd, Tb, Dy, Ho, Fr, Tm)
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              197
_journal_page_last               207
_journal_volume                  31
_journal_year                    1980
_chemical_formula_sum            'Pt Tb'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.013
_cell_length_b                   4.49
_cell_length_c                   5.564
_cell_volume                     175.201
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Castets_JSSCBI_1980_1298.cif
_cod_data_source_block           Pt1Tb1
_cod_original_cell_volume        175.2013
_cod_original_formula_sum        'Pt1 Tb1'
_cod_database_code               1523377
Magnetic properties and structure of Tb2 Pt
Castets, A.; Roudaut, E.; Gomez-Sal, J.C.; Gignoux, D.; Rodriguez-Gonzales, F.; Physica Status Solidi, Sectio A: Applied Research 73 (1982) 475–481; doi:

data_1523378
_publ_section_title
;
 Magnetic properties and structure of Tb2 Pt
;
_journal_name_full
'Physica Status Solidi, Sectio A: Applied Research'
_journal_page_first              475
_journal_page_last               481
_journal_volume                  73
_journal_year                    1982
_chemical_formula_sum            'Pt Tb2'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.147
_cell_length_b                   4.772
_cell_length_c                   8.763
_cell_volume                     298.866
_citation_journal_id_ASTM        PSSABA
_cod_data_source_file            Castets_PSSABA_1982_1851.cif
_cod_data_source_block           Pt1Tb2
_cod_original_cell_volume        298.8663
_cod_original_formula_sum        'Pt1 Tb2'
_cod_database_code               1523378
Magnetic properties and structures of Pr Pt and Nd Pt
Castets, A.; Gignoux, D.; Gomez-Sal, J.C.; Roudaut, E.; Solid State Communications 44 (1982) 1329–1334; doi:

data_1523379
_publ_section_title
;
 Magnetic properties and structures of Pr Pt and Nd Pt
;
_journal_name_full               'Solid State Communications'
_journal_page_first              1329
_journal_page_last               1334
_journal_volume                  44
_journal_year                    1982
_chemical_formula_sum            'Nd Pt'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   3.846
_cell_length_b                   10.769
_cell_length_c                   4.542
_cell_volume                     188.119
_citation_journal_id_ASTM        SSCOA4
_cod_data_source_file            Castets_SSCOA4_1982_1434.cif
_cod_data_source_block           Nd1Pt1
_cod_original_cell_volume        188.1186
_cod_original_formula_sum        'Nd1 Pt1'
_cod_database_code               1523379